# Material Science. Prof. Satish V. Kailas Associate Professor Dept. of Mechanical Engineering, Indian Institute of Science, Bangalore India

Save this PDF as:

Size: px
Start display at page:

Download "Material Science. Prof. Satish V. Kailas Associate Professor Dept. of Mechanical Engineering, Indian Institute of Science, Bangalore 560012 India"

## Transcription

1 Material Science Prof. Satish V. Kailas Associate Professor Dept. of Mechanical Engineering, Indian Institute of Science, Bangalore India Chapter 14. Electrical properties Engineering materials are important in everyday life because of their versatile structural properties. Other than these properties, they do play an important role because of their physical properties. Prime physical properties of materials include: electrical properties; thermal properties; magnetic properties; and optical properties. The electrical behaviors of engineering materials are diverse, and so are their uses in electrical applications. Few examples of electrical applications: copper and aluminium wires used in power transmission; amorphous silicon in solar cells; LEDs; gallium-arsenide chips used in modern day computers, cell phones, digital assistants; etc. This chapter shall describe electrical properties and behavior of engineering materials in electrical applications. First, basic electrical property, electrical conductivity, will be described followed by different types of electrical conduction including semi- and superconductivities. Some peculiar phenomena like ferro-electricity and peizo-electricity are explained in addition to electrical insulation Electrical conduction Electrical conductivity of a material is defined in terms of ease with which a material transmits an electrical current. Electrical current (I) is flow of electrons, and driving force for the flow of electrons is called voltage (V). Ohm s law relates these parameters as follows: V α I V = IR...(1) where R is the materials resistance to flow of electrons through it. V, I, and R respectively have units as volts, amperes, and ohms (Ω).

2 Electrical resistance of a material is influenced by its geometric configuration; hence a new parameter called electrical resistivity (ρ) is defined such as it is independent of the geometry. ρ = RA l...(2) where A cross-sectional area perpendicular to the direction of the current, and l the distance between points between which the voltage is applied. Units for ρ are ohm-meters (Ω-m). Reciprocal of the electrical resistivity, known as electrical conductivity (σ), is used to express the electrical behavior of a material, which is indicative of the ease with which a material allows of flow of electrons. 1 σ = = ρ l RA....(3) Electrical conductivity has the following units: (Ω-m) -1 or mho/meter. Resistivity or conductivity does not depend on the dimensions of the material. These properties are microstructure-sensitive instead, like many other intrinsic properties, for example yield strength. Thus either of it (usually conductivity) allows us to compare different materials. Solid engineering materials exhibit very wide range of electrical conductivity (about 27 orders of variation). Hence the materials for electrical applications are classified according to their electrical conductivity as: conductors, semiconductors and insulators/dielectrics. Metals are conductors having conductivities in range of 10 7 (Ω-m) -1, while semiconductors have conductivities in range from 10-6 to 10 4 (Ω-m) -1, and materials with conductivity lower than (Ω-m) -1 are termed as insulators. In components designed to conduct electrical energy, minimizing losses is important to conserve energy as well as minimize heating. The electric power (P) lost when a current flows through a material is given by: P = VI = I 2 R..(4) Electrical losses are also known as Joule heating losses. Second form of Ohm s law can be obtained by combining the equations (3) and (4) to give: I A V = σ J = σe (5) l where J current density (A/cm 2 ), E electric field strength (V/cm).

3 Current density can be defined in different terms as J = n. q. v..(6) where n number of charge carriers (1/cm 3 ), q charge on each carrier (1.6x10-19 C), v - average drift velocity (cm/s), which occurs as a result of an applied electric or magnetic field. The term v /E is called mobility, μ (cm 2 /V.s) of the carriers, thus σ = n.q.μ.(7) From the above equation, the following can be concluded: electrical conductivity of a material can be controlled by (i) controlling number of charge carriers, n or (ii) controlling the mobility of the carriers, μ. Mobility is important for metals or electrical conductors, whereas number of carriers is important for semi-conductors and insulators. Electrons are charge carriers in metals. In ionic materials (for example ionic ceramics), conduction is result of net movement of charged particles (cations and anions) in addition to any electron motion. However, both electrons and holes are charge carriers in semiconductors and in doped conductive polymers. Thus equation 7 can be written as follows: for metals : σ = ne. q e. μe (8) for semiconductors : σ = n. q. μn + n. q. μ p..(9) for ionic materials : σ total = σ electronic + σ ionic.(10) In all conductors, semiconductors, and many insulating materials, only electronic conduction exists i.e. electrons are the only charge carriers. Ionic conduction results because of net motion of charged ions. Movement different particles in various materials depend on more than one parameter. These include: atomic bonding, imperfections, microstructure, ionic compounds, diffusion rates and temperature. Because of these, electrical conductivity of materials varies tremendously. In metals not all electrons will accelerate in the presence of an electric field. Instead the number of charge carriers is dependent on the arrangement of electron states/levels with respect to energy, and the manner in which these states are occupied by electrons. Electrons in metals are arranged into shells and sub-shells in accordance with Pauli exclusion principle. Each of these shells / sub-shells is distinguished from every other by their energy state/level. Basic existence of metals is dependent on metallic bond where large groups of atoms come together and share valence electrons in what is called metallic bond. Thus there are N atoms in the lattice with N atomic orbitals and N

4 molecular orbitals, many of which are of same energy. This leads to bands of electrons. The electrons not involved in bonding remain in what is called the core band, whereas the valence electrons that form the electron gas enter into the valence band. The remaining un-filled orbitals form higher-energy bands, called conduction band. It is the conduction band that gives metals and alloys the ability to freely conduct electrons. Four different types of band structures are possible at 0 K: (1) Where one outermost band is only partially filled with electrons. The energy corresponding to the highest filled state at 0 K is called the Fermi energy, E f. (2) There is overlap of an empty band and a filled band. (3) and (4) One filled band (valence band) and an empty band (conduction band) are separated by an energy band gap which lies between them. These are schematically shown in the figure Figure 14-1: Possible electron band structures. Band structures (1) and (2) are found in metals / conductors. Band structures (3) and (4) are distinguished by the size of energy band gap. Narrower energy band gap i.e. size < 2 ev, is found in semiconductors, while the broader energy band gap i.e. size > 4 ev, is found in insulators. Fermi energy for these two band structures lies within the band gap near its center. Metals have high conductivities because of the large number of free electrons that have been excited into empty states above the Fermi energy. If the metal crystal lattices were perfect and there are no lattice vibrations, the electrons would pass through the lattice unscattered, encountering no resistance. However, lattice vibrations and phonon scattering play a role in disrupting the mean free path of electrons. In addition, crystalline defects and impurity atom affect the conductivity. These scattering mechanisms act independently on one another. Thus the effective resistivity of metals can be represented as follows:

5 ρ = ρ thermal + ρ residual...(11) Equation 11 is some times known as Mathiessen s rule. With increase of temperature, thermal vibrations increase so the resistivity, and vice versa. In the same manner, with increase of either defects or impurities, resistivity increases. Thus, in general, for pure metals, the resistivity approaches zero at absolute zero temperature. Some metals, however, such as Pb, lose all resistivity abruptly and completely at some low temperatures. This phenomenon is called superconductivity, and the materials that exhibit it are called superconductors. The temperature at which the resistivity vanishes is called the critical transition temperature, T c. Many elemental metals, solid-solution alloys, some ceramics and intermetallic compounds exhibit superconductivity. For example: Ti, V, Zn, W, Al, Hg, NbTi, Nb 3 Sn, MgB 2, La-Sr-Cu oxide, YBa 2 Cu 3 O 7-x, carbon nanotubes, etc. BCS (Bardeen, Cooper and Schrieffer) theory explains that the super conductivity is caused by electron-lattice interaction and that the superconducting electrons consist of paired ordinary electrons called a Cooper pair Semiconductivity Conductivity of semiconductors is not as high as metals / conductors. However, their electrical properties are unique, in the sense that their electrical properties are extremely sensitive to even minute concentrations of impurities. For intrinsic semiconductors, their electrical behavior is based on inherent electronic structure of the pure material. On the other hand, if the electrical properties are dominated by impurities, they are called extrinsic semiconductors. Intrinsic semiconduction: Energy band gap between the valence and conduction bands can be used to classify materials as conductors, insulators, and semiconductors. The magnitude of the band gap is characteristic of the lattice alone, and varies widely for different crystals. In semiconductors, the valence and conduction bands do not overlap as in metals, but they possess enough electrons in the valence band those can be promoted to the conduction band at a certain temperature. Promotion of electrons leaves behind positively charged holes in the valence band which maintain the charge neutrality. These holes can be regarded as moving positive charges through the crystal with a charge magnitude and ass as that of an electron. Conduction that arises from thermally / optically excited electrons is called intrinsic semiconduction. It usually takes place at elevated temperatures since sufficient thermal agitation is necessary to transfer a reasonable number of electrons from the valence band to the conduction band. At still higher temperatures, the concentration of thermally excited electrons in the conduction band becomes so high that the semiconductor behaves more like a metal. The elements capable of intrinsic conduction are limited, and include: Si, Ge, Sn, Pb, etc.

6 Figure 14-2: Band structure and intrinsic conductivity. In intrinsic semiconductors, the number of holes equals the number of mobile electrons. The resulting conductivity can be expressed as σ = n q. μ + n. q. μ = n. q.( μ + μ )..(12) e. e e h h h e e e h as n e = n h, and both electron and hole possess equal magnitude of charge. The mobility of holes is always less than those of electrons i.e. μ h < μ e. In Si and Ge, the ratio μ e / μ h is approximately three and two respectively. Extrinsic semiconduction: The charge carrier density can also be increased by adding impurities of either higher or lower valence. This addition of impurities is known as doping, and impure atoms in the element are called donor atoms. When a pentavalent substitutional atoms like P, As, or Sb are placed into a covalently bonded tetravalent materials such as Si or Ge, only four of their five valence electrons are required to participate in covalent bonding, while the fifth electron remains weakly bound to the donor atom. However, this binding energy is in order of 0.01 ev, much less than that of a covalently bonded electron. The energy state of this electron is indicated as E d. Energy gap between the donor and conducting bands is much smaller than that between the valence band and conduction band, E g. Thermal agitation, even at room temperature, is good enough to excite this electron to the conduction band, leaving behind a positively charged hole in the donor band. Conductivity is due to motion of negatively charged electrons in the conduction band, and so the material is called n-type semiconductor. Fermi level (E f ) of n-type extrinsic semiconductor is higher than that of intrinsic semiconductor i.e. it shifted upward in the band gap, to within the vicinity of the donor state; and its exact position is a function of both temperature and donor concentration.

7 Figure 14-3: Band structure and n-type semiconductivity. Other possibility of susbstituion involves impurity with lower valence. For example trivalent elements like B, Al, Ga, In, Th doped to Si or Ge. Since the donor atoms are deficient in bonding electrons, one of their bonding orbitals will contain a hole that is capable of accepting an electron from elsewhere in the crystal. Binding energy is small, and promotion of an electron from the valence band to the acceptor band, E a, leaves a positively charged hole in the valence band that can act as a charge carrier. Materials with this p-type extrinsic semiconduction are called p-type semiconductors. Fermi level (E f ) for p-type semiconductors is positioned within the band gap and near to the acceptor level. Figure 14-4: Band structure and p-type semiconductivity. For an n-type semiconductor, electrons in the conduction band are charge carriers and holes participate in bonding, whereas for a p-type semiconductor, the electrons participate in bonding, and the holes are the charge carriers. Conductivity equations for these extrinsic semiconductors are written as: n-type semiconductor: p-type semiconductor: σ n. q. μ.(13) e σ n. q. μ..(14) h

8 In both types of extrinsic semiconductors, the doping elements are chosen so that both acceptor and donor levels are located closer to the corresponding energy bands and only a small energy gap in involved when exciting electrons. Intrinsic semiconductors are pure to the order greater than 10 7, while extrinsic semiconductors are made with impurity levels in order of ppm. In intrinsic semiconductors, the conductivity is dominated by the exponential relation between temperature and band-gap. However, the conductivity of extrinsic semiconductors is governed by competing forces: charge carrier density and charge carrier mobility. At low temperatures, the number of charge carriers initially increases with temperature. At intermediate temperatures, for n-type extrinsic semiconductor, most of the donor electrons have been promoted and the number of charge carriers is nearly independent of temperature in what is known as the exhaustion range. At higher temperatures, the number of valence electrons excited to the conduction band greatly exceeds the total number of electrons from the donor atoms, and extrinsic semiconductor behaves like an intrinsic semiconductor. That is, at low temperatures the conductivity varies with temperature as the charge carrier concentration, at higher temperatures the charge carrier mobility dominates and the conductivity decreases with temperature, and at still higher temperatures the extrinsic semiconductor behaves like an intrinsic semiconductor Electrical conduction in ionic ceramics and in polymers In addition to the conduction of charge via electrons, charge can be conducted via ions. Ions are present in most crystalline ceramic materials such as oxides and halides. This process is called ionic conduction, and may occur either in conjunction with or separately from electronic conduction. Several types of compounds show exceptionally high ionic conductivity. Such phases fall into three broad categories: halide and chalcogenides of silver and copper; oxides with β- alumina structure; and oxides of fluorite structure. Conductivity of halides and chalcogenides is result of larger number of available sites than the number of cations. In oxides with β-alumina structure (AM 11 O 17 ) monovalent cation A (such as Na, K, Rb, Li) is mobile. High dopant levels in the fluorite-type solid solutions leads to large defect concentrations and vacancy ordering which results in rapid oxygen migrations. This is the base for development of high-temperature superconductors. For example: La 2 CuO 4 (T c = 30 K), YBC compounds yttrium doped perovskite structure, YBa 2 Cu 3 O 7 (T c = 92 K). Although ceramics are insulators, by properly engineering the point defects in ceramics, it is possible to convert them into semiconductors. For example: Indium tin oxide (ITO) is used as a transparent conductive coating on plate glass, and also for tough screen displays; Ytrria-stabilized zirconia (YSZ) is used as solid electrolyte in solid oxide fuel cells; Lithium cobalt oxide is used as solid electrolyte in lithium ion batteries. Polymers have a band structure with a large energy gap leading to low conductivity because their valence electrons are involved in covalent boding. Hence polymers are used

9 frequently in applications that require electrical insulation. In some cases however, low conductivity is undesirable. For example; static electricity can accumulate on housing for electronic equipment making the polymer vulnerable to electromagnetic radiation that damages the internal devices. These problems can be solved in two approaches: (1) introducing an additive to the polymer to improve conductivity, and (2) creating polymers with inherent conductivity. Adding ionic compound to the polymer can reduce resistivity because the ions migrate to the polymer surface and attract moisture, which in turn, dissipates static charges. Introducing conductive fillers such as carbon black can also dissipate static charges. Some polymers inherently have good conductivity as result of doping or processing techniques. When acetal polymers are doped with agents such as arsenic pentafluoride, electrons or holes are able to jump freely from one atom to another along the backbone of the chain, increasing the conductivity to near that of metals. However, unlike semiconductors, the dopant atoms or molecules do not substitute for or replace the polymer atoms. Other polymers include polyparaphynylene, polypyrole, and polyaniline. Some other polymers such as polyphthaocyanine can be cross-linked by special curing processes to raise its conductivity Dielectric behavior A dielectric is a material separating two charged bodies. For a material to be a good dielectric, it must be an electrical insulator. Thus, any insulator is also called a dielectric. Dielectric materials are used in capacitors, devices used to store the electric energy. When a voltage is applied between two parallel plates in a vacuum, one plate becomes positively charged and the other negatively charged, with corresponding field directed from the positive to the negative. Then the energy stored, Q, is given by: Q = CV... (15) where C is the capacitance (units: coulombs per volt or farads [F]). It is dependent on the geometry of plates as follows: A C = ε 0.. (16) l where A area of the plates, l distance between them, and ε 0 permittivity of vacuum (8.85 X F/m). If a dielectric material is inserted between the plates, A C = ε. (17) l ε permittivity of the medium, which will be greater in magnitude than ε 0. The relative permittivity ε r, also called dielectric constant, is defined as

10 ε ε r =...(18) ε 0 which is greater than unity, and presents the increase in charge storing capacity by insertion of the dielectric medium between the plates. This is result of polarization orientation of permanent or induced dipoles under externally applied electric field. Polarization causes positive charge to accumulate on the bottom surface next to the negatively charged plate, and causes negative charge to accumulate toward the positively charged plate on the top. This tends to decrease the effective surface charge density on either plate. The expected decrease in effective charge corresponds to the polarization, of the material which equals the induced dipole moment per unit volume of polarizable material. The magnitude of the charge per unit area on either plate, called the dielectric displacement or flux density or surface charge density, D, is defined as: D = εξ. (19) where ξ electric field strength, ξ = V / l.. (20) In the presence of the dielectric, surface charge density can also be presented as D = εξ = ε 0 ξ + P (21) where polarization is defined as, P ε ( ε 1) ξ... (22) = 0 r the increase in charge density above that for a vacuum because of the presence of the dielectric. Figure 14-5: Schematic representation of capacitor and polarization phenomenon.

11 The polarization may also be thought of as the total dipole moment per unit volume of the dielectric material or as a polarization electric field within the dielectric that results from the mutual alignment of the many a atomic or molecular dipoles. Polarization of a dielectric material may be caused by at least one of four major types of polarization: electronic, ionic (atomic), orientation, and space charge (interfacial). Electronic polarization arises because the center of the electron cloud around a nucleus is displaced under an applied electric field. Ionic polarization occurs in ionic materials because an applied field acts to displace cations in the direction of the applied field while displacing anions in a direction opposite to the applied field. Orientation polarization can occur in materials that possess permanent electric dipole moments. These permanent dipoles tend to become aligned with the applied electric field, but entropy and thermal effects tend to counter this alignment, thus it is highly temperature dependent. Space charge polarization results from the accumulation of charge at structural interfaces in heterogeneous materials. Such polarization occurs when one of the phases has a much higher resistivity than the other. The total polarization subjected to an alternating electric field depends upon the ease with which the permanent or induced dipoles can reverse their alignment. The time required for dipole reversal is called the relaxation time, and its reciprocal is called the relexation frequency. As the frequency of the applied electric field approached the relaxation frequency, the polarization response increasingly lags behind the applied field. The reorientation of each type of dipole is opposed by internal friction, which leads to heating in the sample and power loss. The power loss depends on the degree to which the polarization lags behind the electric field. This is also called dielectric loss, and a low dielectric loss is desired at the frequency of utilization. At high enough frequencies, the dielectric will experience electrical breakdown initiated by the field-induced excitation of a number of electrons into the conduction band, and the insulator become a conductor. The magnitude of the electric field required to cause dielectric breakdown is called the dielectric strength or breakdown strength. Many ceramics and polymers are utilized as insulators and in capacitors. For example: glass, porcelain, stealite, mica. These have dielectric constants within the range of Typical applications: electrical insulation, switch bases, light receptacles. Dielectric constant for most polymers lies in the range of 2-5, less than that for ceramics, since the later exhibit greater dipole moments. Typical applications: insulation for wires, cables, motors, generators, some capacitors Ferro-electricity and Piezoelectricity Two peculiar phenomena related to electric dipoles are ferro-electricity and piezoelectricity. Ferro-electricity is defined as the spontaneous alignment of electric dipoles by their mutual interaction in the absence of an applied electric field. This arises from the fact that the local field increases in proportion to the polarization. Thus, ferro-electric materials must possess permanent dipoles. Ex.: BaTiO 3, Rochelle salt

12 (NaKC 4 H 4 O 6.4H 2 O), potassium dihydrogen phosphate (KH 2 PO 4 ), potassium niobate (KNbO 3 ). These materials have extremely high dielectric constants at relatively low applied field frequencies. Thus, capacitors made from ferro-electric materials are smaller than capacitors made of other dielectric materials. Piezo-electricity, or pressure electricity, is defined as polarization induced by the application of external force. Hence, by reversing the direction of external force, direction of the field can be reversed i.e. the application of an external electric field alters the net dipole length and causes a dimensional change. This property is characteristic of materials having complicated structures with a low degree of symmetry. Thus, piezoelectric materials can be used as transducers devices that convert mechanical stress into electrical energy and vice versa. Application for these materials includes microphones, ultrasonic generators, sonar detectors, and mechanical strain gauges. Ex.: Barium titanate, lead titanate, lead zirconate (PbZrO 3 ), ammoinium dihydrogen phosphate (NH 4 H 2 PO 4 ), and quartz. References 1. W. D. Kingery, H. K. Bowen, and D. R. Uhlmann, Introduction to Ceramics, Second Edition, Wiley, New York, R. E. Hummel, Electronic Properties of Materials, Third Edition, Springer-Verlag, New York, William D. Callister, Jr, Materials Science and Engineering An introduction, sixth edition, John Wiley & Sons, Inc

### Basic laws and electrical properties of metals (I) Electrical properties. Basic laws and electrical properties of metals (II)

Electrical properties Electrical conduction How many moveable electrons are there in a material (carrier density)? How easily do they move (mobility)? Semiconductivity Electrons and holes Intrinsic and

### MCEN Fall 2003.

Basic types of solid materials. Overview The theory of bands provides a basis for understanding the classification and physical properties of solid materials such as electrical conductivity, optical behavior

### Module 6 : PHYSICS OF SEMICONDUCTOR DEVICES Lecture 34 : Intrinsic Semiconductors

Module 6 : PHYSICS OF SEMICONDUCTOR DEVICES Lecture 34 : Intrinsic Semiconductors Objectives In this course you will learn the following Intrinsic and extrinsic semiconductors. Fermi level in a semiconductor.

### Electrical Properties

Electrical Properties Outline of this Topic 1. Basic laws and electrical properties of metals 2. Band theory of solids: metals, semiconductors and insulators 3. Electrical properties of semiconductors

### phys4.17 Page 1 - under normal conditions (pressure, temperature) graphite is the stable phase of crystalline carbon

Covalent Crystals - covalent bonding by shared electrons in common orbitals (as in molecules) - covalent bonds lead to the strongest bound crystals, e.g. diamond in the tetrahedral structure determined

### Semiconductors, diodes, transistors

Semiconductors, diodes, transistors (Horst Wahl, QuarkNet presentation, June 2001) Electrical conductivity! Energy bands in solids! Band structure and conductivity Semiconductors! Intrinsic semiconductors!

### Condensed Matter Physics Prof. G. Rangarajan Department of Physics Indian Institute of Technology, Madras. Lecture - 36 Semiconductors

Condensed Matter Physics Prof. G. Rangarajan Department of Physics Indian Institute of Technology, Madras Lecture - 36 Semiconductors We will start a discussion of semiconductors one of the most important

### - thus the electrons are free to change their energies within the 3s band

Allowed and Forbidden Energy Bands - allowed energy bands associated with different atomic orbitals may overlap, as in (a) - the regions between allowed energy bands are called forbidden bands or band

### Material Science. Prof. Satish V. Kailas Associate Professor Dept. of Mechanical Engineering, Indian Institute of Science, Bangalore India

Material Science Prof. Satish V. Kailas Associate Professor Dept. of Mechanical Engineering, Indian Institute of Science, Bangalore 5612 India Chapter 15. Thermal properties Engineering materials are important

### Doped Semiconductors. Dr. Katarzyna Skorupska

Doped Semiconductors Dr. Katarzyna Skorupska 1 Doped semiconductors Increasing the conductivity of semiconductors by incorporation of foreign atoms requires increase of the concentration of mobile charge

### Crystalline solids. A solid crystal consists of different atoms arranged in a periodic structure.

Crystalline solids A solid crystal consists of different atoms arranged in a periodic structure. Crystals can be formed via various bonding mechanisms: Ionic bonding Covalent bonding Metallic bonding Van

### ELECTRONIC DEVICES MENJANA MINDA KREATIF DAN INOVATIF

INTRODUCTION TO ELECTRONIC DEVICES MENJANA MINDA KREATIF DAN INOVATIF Introduction What is Electronics? Electronic Devices? Electronic Systems? introduction Electronics: The branch of physics that deals

### Solid State Detectors = Semi-Conductor based Detectors

Solid State Detectors = Semi-Conductor based Detectors Materials and their properties Energy bands and electronic structure Charge transport and conductivity Boundaries: the p-n junction Charge collection

### Analog & Digital Electronics Course No: PH-218

Analog & Digital Electronics Course No: PH-218 Lecture 1: Semiconductor Materials Course Instructors: Dr. A. P. VAJPEYI Department of Physics, Indian Institute of Technology Guwahati, India 1 Semiconductors

### DO PHYSICS ONLINE. conduction band. ~ 6 ev. Fig. 1. Energy band diagram for diamond (insulator) and silicon (semiconductor).

DO PHYSIS ONLINE FROM IDEAS TO IMPLEMENTATION 9.4.3 ATOMS TO TRANSISTORS SEMIONDUTORS ENERGY BANDS Diamond is a very good insulator. The electronic configuration in the ground state is 1s 2 2s 2 2. It

### Lecture 2: Semiconductors: Introduction

Lecture 2: Semiconductors: Introduction Contents 1 Introduction 1 2 Band formation in semiconductors 2 3 Classification of semiconductors 5 4 Electron effective mass 10 1 Introduction Metals have electrical

### 3. Diodes and Diode Circuits. 3. Diodes and Diode Circuits TLT-8016 Basic Analog Circuits 2005/2006 1

3. Diodes and Diode Circuits 3. Diodes and Diode Circuits TLT-8016 Basic Analog Circuits 2005/2006 1 3.1 Diode Characteristics Small-Signal Diodes Diode: a semiconductor device, which conduct the current

### Solid-State Physics: The Theory of Semiconductors (Ch. 10.6-10.8) SteveSekula, 30 March 2010 (created 29 March 2010)

Modern Physics (PHY 3305) Lecture Notes Modern Physics (PHY 3305) Lecture Notes Solid-State Physics: The Theory of Semiconductors (Ch. 10.6-10.8) SteveSekula, 30 March 2010 (created 29 March 2010) Review

### Definition : Characteristics of Metals :

Metallic Bond Definition : It may be defined as, 1. The force that binds a metal ion to a number of electrons with in its sphere of influence. 2. The attractive force which holds the atoms of two or more

### Lecture 8: Extrinsic semiconductors - mobility

Lecture 8: Extrinsic semiconductors - mobility Contents Carrier mobility. Lattice scattering......................... 2.2 Impurity scattering........................ 3.3 Conductivity in extrinsic semiconductors............

### Electrical Conductivity

Advanced Materials Science - Lab Intermediate Physics University of Ulm Solid State Physics Department Electrical Conductivity Translated by Michael-Stefan Rill January 20, 2003 CONTENTS 1 Contents 1 Introduction

### Electronic Structure and the Periodic Table Learning Outcomes

Electronic Structure and the Periodic Table Learning Outcomes (a) Electronic structure (i) Electromagnetic spectrum and associated calculations Electromagnetic radiation may be described in terms of waves.

### ELECTRICAL CONDUCTION

Chapter 12: Electrical Properties Learning Objectives... How are electrical conductance and resistance characterized? What are the physical phenomena that distinguish conductors, semiconductors, and insulators?

### INSTITUTE FOR APPLIED PHYSICS Physical Practice for Learners of Engineering sciences Hamburg University, Jungiusstraße 11

INSTITUTE FOR APPIED PHYSICS Physical Practice for earners of Engineering sciences Hamburg University, Jungiusstraße 11 Hall effect 1 Goal Characteristic data of a test semiconductor (Germanium) should

### This is the 11th lecture of this course and the last lecture on the topic of Equilibrium Carrier Concentration.

Solid State Devices Dr. S. Karmalkar Department of Electronics and Communication Engineering Indian Institute of Technology, Madras Lecture - 11 Equilibrium Carrier Concentration (Contd.) This is the 11th

### Matter, Materials, Crystal Structure and Bonding. Chris J. Pickard

Matter, Materials, Crystal Structure and Bonding Chris J. Pickard Why should a theorist care? Where the atoms are determines what they do Where the atoms can be determines what we can do Overview of Structure

### Chapter 16. Diodes and Applications. Objectives

Chapter 16 Diodes and Applications Objectives Understand the basic structure of semiconductors and how they conduct current Describe the characteristics and biasing of a pn junction diode Describe the

### Intrinsic and Extrinsic Semiconductors, Fermi-Dirac Distribution Function, the Fermi level and carrier concentrations

ENEE 33, Spr. 09 Supplement I Intrinsic and Extrinsic Semiconductors, Fermi-Dirac Distribution Function, the Fermi level and carrier concentrations Zeynep Dilli, Oct. 2008, rev. Mar 2009 This is a supplement

### Understanding the p-n Junction by Dr. Alistair Sproul Senior Lecturer in Photovoltaics The Key Centre for Photovoltaic Engineering, UNSW

Understanding the p-n Junction by Dr. Alistair Sproul Senior Lecturer in Photovoltaics The Key Centre for Photovoltaic Engineering, UNSW The p-n junction is the fundamental building block of the electronic

### PIEZO CERAMICS. Noliac Group develops and manufactures piezoelectric. zirconate titanate (PZT) of high quality and tailored for custom

Noliac Group develops and manufactures piezoelectric zirconate titanate (PZT) of high quality and tailored for custom Piezoelectric components may be used as e.g.: Actuators Sensors Generators Transducers

### Free Electron Fermi Gas (Kittel Ch. 6)

Free Electron Fermi Gas (Kittel Ch. 6) Role of Electrons in Solids Electrons are responsible for binding of crystals -- they are the glue that hold the nuclei together Types of binding (see next slide)

### - in a typical metal each atom contributes one electron to the delocalized electron gas describing the conduction electrons

Free Electrons in a Metal - in a typical metal each atom contributes one electron to the delocalized electron gas describing the conduction electrons - if these electrons would behave like an ideal gas

### Chapter 3 Atomic Structure and Properties

Chapter 3 Atomic Structure and Properties Introduction The nuclear atom and quantum theory are the accepted theories for the atom. In this chapter, we demonstrate their utility by using them to explain

### Physics 551: Solid State Physics F. J. Himpsel

Physics 551: Solid State Physics F. J. Himpsel Background Most of the objects around us are in the solid state. Today s technology relies heavily on new materials, electronics is predominantly solid state.

### PS-6.2 Explain the factors that determine potential and kinetic energy and the transformation of one to the other.

PS-6.1 Explain how the law of conservation of energy applies to the transformation of various forms of energy (including mechanical energy, electrical energy, chemical energy, light energy, sound energy,

### Magnetic and Dielectric Properties of Solids

Magnetic and Dielectric Properties of Solids Magnetic Properties Some definitions: Paramagnetism: unpaired electrons on some atoms, random orientations of electron spins with each other. Spins align in

### 3. What would you predict for the intensity and binding energy for the 3p orbital for that of sulfur?

PSI AP Chemistry Periodic Trends MC Review Name Periodic Law and the Quantum Model Use the PES spectrum of Phosphorus below to answer questions 1-3. 1. Which peak corresponds to the 1s orbital? (A) 1.06

### Chapter 5. Second Edition ( 2001 McGraw-Hill) 5.6 Doped GaAs. Solution

Chapter 5 5.6 Doped GaAs Consider the GaAs crystal at 300 K. a. Calculate the intrinsic conductivity and resistivity. Second Edition ( 2001 McGraw-Hill) b. In a sample containing only 10 15 cm -3 ionized

### Classes of materials

Classes of materials POLYMERS CERAMICS METALS DUCTILITY Varies Poor Good CONDUCTIVITY (ELECTRICAL & THERMAL) Low Low High HARDNESS/STRENGTH Low medium Very high Medium high CORROSION RESISTANCE Fair good

### The Physics of Energy sources Renewable sources of energy. Solar Energy

The Physics of Energy sources Renewable sources of energy Solar Energy B. Maffei Bruno.maffei@manchester.ac.uk Renewable sources 1 Solar power! There are basically two ways of using directly the radiative

### 1.5 Light absorption by solids

1.5 Light absorption by solids Bloch-Brilloin model L e + + + + + allowed energy bands band gaps p x In a unidimensional approximation, electrons in a solid experience a periodic potential due to the positively

### Capacitance and Ferroelectrics

Ram Seshadri MRL 2031, x6129 seshadri@mrl.ucsb.edu; http://www.mrl.ucsb.edu/ seshadri/teach.html Capacitance and Ferroelectrics A voltage V applied across a capacitor of caacitance C allows a quantity

### Lecture 2 Semiconductor Physics (I)

Lecture 2 Semiconductor Physics (I) Outline Intrinsic bond model : electrons and holes Generation and recombination Intrinsic semiconductor Doping: Extrinsic semiconductor Charge Neutrality Reading Assignment:

### University of Toronto Department of Electrical and Computer Engineering. ECE 330F SEMICONDUCTOR PHYSICS Eng. Annex 305

University of Toronto Department of Electrical and Computer Engineering ECE 330F SEMICONDUCTOR PHYSICS Eng. Annex 305 Experiment # 1 RESISTIVITY AND BAND GAP OF GERMANIUM TA: Iraklis Nikolalakos OBJECTIVE

### Introduction to Electricity & Magnetism. Dr Lisa Jardine-Wright Cavendish Laboratory

Introduction to Electricity & Magnetism Dr Lisa Jardine-Wright Cavendish Laboratory Examples of uses of electricity Christmas lights Cars Electronic devices Human body Electricity? Electricity is the presence

### Tunnel Diode. - in a heavily doped p-n junction the depletion region is very small (~ 10 nm)

Tunnel Diode - in a heavily doped p-n junction the depletion region is very small (~ 10 nm) - the bottom of the n-side conduction band overlaps the p-side valence band, see (a) - with a small forward bias

### Semiconductor Physics

10p PhD Course Semiconductor Physics 18 Lectures Nov-Dec 2011 and Jan Feb 2012 Literature Semiconductor Physics K. Seeger The Physics of Semiconductors Grundmann Basic Semiconductors Physics - Hamaguchi

### CHEM 10113, Quiz 7 December 7, 2011

CHEM 10113, Quiz 7 December 7, 2011 Name (please print) All equations must be balanced and show phases for full credit. Significant figures count, show charges as appropriate, and please box your answers!

### The Piezoelectric Effect, Ferroelectricity, the Photoelectric Effect, and why Metals Are Shiny

Physics 5K Lecture Friday Apr 27, 2012 The Piezoelectric Effect, Ferroelectricity, the Photoelectric Effect, and why Metals Are Shiny Joel Primack Physics Department UCSC Piezoelectric Effect Sqeezing

### Crystal Chemistry. This document last updated on 22-Sep-2014

Page 1 of 14 EENS 2110 Tulane University Crystal Chemistry Mineralogy Prof. Stephen A. Nelson This document last updated on 22-Sep-2014 As we have been discussing for the last several weeks, crystals,

### Displacement, and Position sensors

Displacement, and Position sensors Displacement Measurement Measurement of displacement is the basis of measuring: Position Velocity Acceleration Stress Force Pressure Proximity Thickness 1 Displacement

### Semiconductors Band Formation & direct and indirect gaps. Prof.P. Ravindran, Department of Physics, Central University of Tamil Nadu, India

Semiconductors Band Formation & direct and indirect gaps 1 Prof.P. Ravindran, Department of Physics, Central University of Tamil Nadu, India http://folk.uio.no/ravi/semi2013 Review of Energy Bands (1)

### An organic semiconductor is an organic compound that possesses similar

MSE 542 Final Term Paper Title: Organic Semiconductor for Flexible Electronics Name: Chunhung Huang Introduction: An organic semiconductor is an organic compound that possesses similar properties to inorganic

### S block elements p block elements and chemical bonding -1

S block elements p block elements and chemical bonding -1 1.Group I elements do not occur free (native state) in the nature because a. They are unstable b. Their compounds with other elements are highly

### Untitled Document. 1. Which of the following best describes an atom? 4. Which statement best describes the density of an atom s nucleus?

Name: Date: 1. Which of the following best describes an atom? A. protons and electrons grouped together in a random pattern B. protons and electrons grouped together in an alternating pattern C. a core

### Semiconductors, Diodes and Their Applications

Chapter 16 Semiconductors, Diodes and Their Applications A diode is a one-way valve for Current Examples of One-Way Valves Air Check Valve Leg Vein Valves Heart Valves Typical diode packages and terminal

### Processing of Semiconducting Materials Prof. Pallab Banerji Material Science Centre Indian Institute of Technology, Kharagpur

Processing of Semiconducting Materials Prof. Pallab Banerji Material Science Centre Indian Institute of Technology, Kharagpur Lecture - 27 Characterization II Let us define the following parameters for

### Topic 4. Chemical bonding and structure

Topic 4. Chemical bonding and structure There are three types of strong bonds: Ionic Covalent Metallic Some substances contain both covalent and ionic bonding or an intermediate. 4.1 Ionic bonding Ionic

### Imperfections in atomic arrangements

MME131: Lecture 8 Imperfections in atomic arrangements Part 1: 0D Defects A. K. M. B. Rashid Professor, Department of MME BUET, Dhaka Today s Topics Occurrence and importance of crystal defects Classification

### Section A5: Current Flow in Semiconductors

Section A5: Current Flow in Semiconductors Conductive behaviors in materials, defined by the parameter conductivity, are a primary factor in the development of electronic and optoelectronic devices. Electrical

### Electro - Principles I

Electro - Principles I Atomic Theory Atomic Theory Page It is our intention here to handle atomic theory in a very light manner. Some knowledge is required in order to understand the characteristics of

### Chapter No: 14 Chapter: Semiconductor Electronics: Materials, Devices And Simple Circuits (ONE MARK QUESTIONS)

Chapter No: 14 Chapter: Semiconductor Electronics: Materials, Devices And Simple Circuits (ONE MARK QUESTIONS) 1. What is an electronic device? It is a device in which controlled flow of electrons takes

### Dielectric Properties of Polymers

TECHNICAL WHITEPAPER Dielectric Properties of Polymers Introduction Understanding the structure of plastics (and in particular, the fluoropolymers) not only gives a better understanding of chemical resistance

### Chapter 18 魏 茂 國. Materials Science and Engineering

Chapter 18 Introduction Ohm s law Electrical conductivity Electronic and ionic conduction Energy band structures in solids Conduction in terms of band and atomic bonding models Electronic mobility Electrical

### Unit 12 Practice Test

Name: Class: Date: ID: A Unit 12 Practice Test Multiple Choice Identify the choice that best completes the statement or answers the question. 1) A solid has a very high melting point, great hardness, and

### Chapter 2. Atomic Structure and Interatomic Bonding

Chapter 2. Atomic Structure and Interatomic Bonding Interatomic Bonding Bonding forces and energies Primary interatomic bonds Secondary bonding Molecules Bonding Forces and Energies Considering the interaction

### Use the PES spectrum of Phosphorus below to answer questions 1-3.

Use the PES spectrum of Phosphorus below to answer questions 1-3. 1. Which peak corresponds to the 1s orbital? (A) 1.06 (B) 1.95 (C) 13.5 (D) 18.7 (E) 208 2. Which peak corresponds to the valence 3p orbital?

### PTC Thermistors [From Philips Data Handbook PA ]

PTC Thermistors [From Philips Data Handbook PA02 1989] 1. GENERAL Positive Temperature Coefficient (PTC) thermistors exhibit a high positive temperature coefficient of resistance. They differ from Negative

### Objectives 200 CHAPTER 4 RESISTANCE

Objectives Explain the differences among conductors, insulators, and semiconductors. Define electrical resistance. Solve problems using resistance, voltage, and current. Describe a material that obeys

### Lecture 2 - Semiconductor Physics (I) September 13, 2005

6.012 - Microelectronic Devices and Circuits - Fall 2005 Lecture 2-1 Lecture 2 - Semiconductor Physics (I) September 13, 2005 Contents: 1. Silicon bond model: electrons and holes 2. Generation and recombination

### Energy Transport. Focus on heat transfer. Heat Transfer Mechanisms: Conduction Radiation Convection (mass movement of fluids)

Energy Transport Focus on heat transfer Heat Transfer Mechanisms: Conduction Radiation Convection (mass movement of fluids) Conduction Conduction heat transfer occurs only when there is physical contact

### Periodic Table. inert gases. Columns: Similar Valence Structure. give up 1e - give up 2e - Oaccept 2e- accept 1e - give up 3e -

Periodic Table give up 1e - give up 2e - give up 3e - H Li Be Na Mg K Ca Columns: Similar Valence Structure Sc Oaccept 2e- accept 1e - inert gases S Se F Cl Br He Ne Ar Kr Adapted from Fig. 2.6, Callister

### Applied Quantum Mechanics for Electrical Engineers Workshop II Energy Band Model and Doping

Applied Quantum Mechanics for Electrical Engineers Workshop II Energy Band Model and Doping 95 pts Objective: Explore the effect of doping on the energy band diagram and the carrier concentration. Instructions:

### COURSE: PHYSICS DEGREE: COMPUTER ENGINEERING year: 1st SEMESTER: 1st

COURSE: PHYSICS DEGREE: COMPUTER ENGINEERING year: 1st SEMESTER: 1st WEEKLY PROGRAMMING WEE K SESSI ON DESCRIPTION GROUPS GROUPS Special room for LECTU PRAC session RES TICAL (computer classroom, audiovisual

### Semiconductors, Insulators and Metals

CHAPTER 2 ENERGY BANDS AND EFFECTIVE MASS Semiconductors, insulators and metals Semiconductors Insulators Metals The concept of effective mass Prof. Dr. Beşire GÖNÜL Semiconductors, Insulators and Metals

### Lecture 3: Optical Properties of Bulk and Nano. 5 nm

Lecture 3: Optical Properties of Bulk and Nano 5 nm The Previous Lecture Origin frequency dependence of χ in real materials Lorentz model (harmonic oscillator model) 0 e - n( ) n' n '' n ' = 1 + Nucleus

### Electronics Field-effect transistors

Electronics Field-effect transistors Prof. Márta Rencz, Gergely Nagy BME DED October 7, 2013 The basics of field-effect transistors The operation of field-effect transistors is based on ability of controlling

### An insulator is a material that has an electrical conductivity in the approximate range of to Ω -1 m -1.

Insulators An insulator is a material that has an electrical conductivity in the approximate range of 10-10 to 10-16 Ω -1 m -1. 1 Insulators Recall: Electronic structure; Band gaps (2-6eV); Range of conductivities;

### KINETIC MOLECULAR THEORY OF MATTER

KINETIC MOLECULAR THEORY OF MATTER The kinetic-molecular theory is based on the idea that particles of matter are always in motion. The theory can be used to explain the properties of solids, liquids,

### SUPERCONDUCTIVITY. PH 318- Introduction to superconductors 1

SUPERCONDUCTIVITY property of complete disappearance of electrical resistance in solids when they are cooled below a characteristic temperature. This temperature is called transition temperature or critical

### CHAPTER 6 Chemical Bonding

CHAPTER 6 Chemical Bonding SECTION 1 Introduction to Chemical Bonding OBJECTIVES 1. Define Chemical bond. 2. Explain why most atoms form chemical bonds. 3. Describe ionic and covalent bonding.. 4. Explain

### Physics Notes Class 12 Chapter 14 Semiconductor Electronics, Materials, Devices and Sample Circuits

1 P a g e Physics Notes Class 12 Chapter 14 Semiconductor Electronics, Materials, Devices and Sample Circuits It is the branch of science which deals with the electron flow through a vacuum, gas or semiconductor.

### 4.1 SOLAR CELL OPERATION. Y. Baghzouz ECE Department UNLV

4.1 SOLAR CELL OPERATION Y. Baghzouz ECE Department UNLV SOLAR CELL STRUCTURE Light shining on the solar cell produces both a current and a voltage to generate electric power. This process requires a material

### Luminescence. Application of luminescence. Dental application. Physical basis of dental material science 11. Optical and other properties.

Luminescence Light emission over the thermal radiation. Light emission after excitation. e.g. atom E 1 Light emission: hn = E 1 E 0 E 0 Excitation: energy uptake by the electron E 0 ground state E 1 excited

### Yrd. Doç. Dr. Aytaç Gören

H2 - AC to DC Yrd. Doç. Dr. Aytaç Gören ELK 2018 - Contents W01 Basic Concepts in Electronics W02 AC to DC Conversion W03 Analysis of DC Circuits W04 Transistors and Applications (H-Bridge) W05 Op Amps

### EDEXCEL NATIONAL CERTIFICATE/DIPLOMA UNIT 5 - ELECTRICAL AND ELECTRONIC PRINCIPLES NQF LEVEL 3 OUTCOME 2 - CAPACITANCE

EDEXCEL NATIONAL CERTIFICATE/DIPLOMA UNIT 5 - ELECTRICAL AND ELECTRONIC PRINCIPLES NQF LEVEL 3 OUTCOME 2 - CAPACITANCE 2 Understand the concepts of capacitance and determine capacitance values in DC circuits

### Atomic Structure. The study of atomic structure is of considerable importance for electronics engineering. 48 Principles of Electronics

48 Principles of Electronics 4 Atomic Structure 4.1 Bohr s Atomic Model 4.2 Energy Levels 4.3 Energy Bands 4.4 Important Energy Bands in Solids 4.5 Classification of Solids and Energy Bands 4.6 Silicon

### Objectives for the standardized exam

III. ELECTRICITY AND MAGNETISM A. Electrostatics 1. Charge and Coulomb s Law a) Students should understand the concept of electric charge, so they can: (1) Describe the types of charge and the attraction

### Solid Type of solid Type of particle

QUESTION (2015:3) Complete the table below by stating the type of solid, the type of particle, and the attractive forces between the particles in each solid. Solid Type of solid Type of particle Cu(s)

### Unit 2 Periodic Behavior and Ionic Bonding

Unit 2 Periodic Behavior and Ionic Bonding 6.1 Organizing the Elements I. The Periodic Law A. The physical and chemical properties of the elements are periodic functions of their atomic numbers B. Elements

### Chapter 26. Capacitance and Dielectrics

Chapter 26 Capacitance and Dielectrics Capacitors Capacitors are devices that store electric charge Examples where capacitors are used: radio receivers filters in power supplies energy-storing devices

### A pure covalent bond is an equal sharing of shared electron pair(s) in a bond. A polar covalent bond is an unequal sharing.

CHAPTER EIGHT BNDING: GENERAL CNCEPT or Review 1. Electronegativity is the ability of an atom in a molecule to attract electrons to itself. Electronegativity is a bonding term. Electron affinity is the

### Lecture 3: Electron statistics in a solid

Lecture 3: Electron statistics in a solid Contents Density of states. DOS in a 3D uniform solid.................... 3.2 DOS for a 2D solid........................ 4.3 DOS for a D solid........................

### Chapter 7: Polarization

Chapter 7: Polarization Joaquín Bernal Méndez Group 4 1 Index Introduction Polarization Vector The Electric Displacement Vector Constitutive Laws: Linear Dielectrics Energy in Dielectric Systems Forces

### Chapter 25: Capacitance

Chapter 25: Capacitance Most of the fundamental ideas of science are essentially simple, and may, as a rule, be expressed in a language comprehensible to everyone. Albert Einstein 25.1 Introduction Whenever

### 21.1 Coulomb s Law - Electric Charge - Conductors and Insulators - Coulomb s law 21.2 Charge is quantized 21.3* Charge is conserved

INTRODUCTION We will understand how electric and magnetic fields affect charged particles Lorentz Force Law: we will learn to describe how electric and magnetic fields are produced by charged particles

### ELECTROSTATICS. Ans: It is a fundamental property of matter which is responsible for all electrical effects

ELECTROSTATICS One Marks Questions with Answers: 1.What is an electric charge? Ans: It is a fundamental property of matter which is responsible for all electrical effects 2. Write the SI unit of charge?

### Chapter 9. Pressure. Pressure. Pressure and Velocity Measurements

Chapter 9 Pressure and Velocity Measurements Material from Theory and Design for Mechanical Measurements; Figliola, Third Edition Pressure Pressure is force per unit area. It acts inward or outward, normal